Strongly Anharmonic Octahedral Tilting in Two-Dimensional Hybrid Halide Perovskites
Menahem, Matan; Dai, Zhenbang; Aharon, Sigalit; Sharma, Rituraj; Asher, Maor; Diskin-Posner, Yael; Korobko, Roman; Rappe, Andrew M.; Yaffe, Omer; ACS Nano  (2021) –; doi:10.1021/acsnano.1c02022

data_4518728
_publ_section_title
;
 Strongly Anharmonic Octahedral Tilting in Two-Dimensional Hybrid Halide
 Perovskites
;
_journal_name_full               'ACS Nano'
_journal_paper_doi               10.1021/acsnano.1c02022
_journal_year                    2021
_chemical_formula_moiety         'I4 Pb, 2(C4 H12 N)'
_chemical_formula_sum            'C8 H24 I4 N2 Pb'
_chemical_formula_weight         863.08
_space_group_crystal_system      orthorhombic
_space_group_IT_number           61
_space_group_name_Hall           '-P 2ac 2ab'
_space_group_name_H-M_alt        'P b c a'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.5057(3)
_cell_length_b                   9.0045(4)
_cell_length_c                   26.6249(12)
_cell_measurement_reflns_used    4253
_cell_measurement_temperature    270(2)
_cell_measurement_theta_max      30.3340
_cell_measurement_theta_min      2.8240
_cell_volume                     2039.19(15)
_computing_cell_refinement       'CrysAlisPro 1.171.40.60a (Rigaku OD, 2019)'
_computing_data_collection       'CrysAlisPro 1.171.40.60a (Rigaku OD, 2019)'
_computing_data_reduction        'CrysAlisPro 1.171.40.60a (Rigaku OD, 2019)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      270(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'XtaLAB Synergy, Dualflex, Pilatus 300K'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0618
_diffrn_reflns_av_unetI/netI     0.0346
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       33
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_number            14997
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.371
_diffrn_reflns_theta_min         1.530
_exptl_absorpt_coefficient_mu    14.313
_exptl_absorpt_correction_T_max  1.000
_exptl_absorpt_correction_T_min  0.900
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.40.60a (Rigaku Oxford Diffraction, 2019)
Numerical absorption correction based on gaussian integration over
			a multifaceted crystal model
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    2.811
_exptl_crystal_description       cube
_exptl_crystal_F_000             1520
_exptl_crystal_size_max          0.094
_exptl_crystal_size_mid          0.084
_exptl_crystal_size_min          0.062
_refine_diff_density_max         1.574
_refine_diff_density_min         -1.574
_refine_diff_density_rms         0.205
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.045
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     72
_refine_ls_number_reflns         2085
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.045
_refine_ls_R_factor_all          0.0527
_refine_ls_R_factor_gt           0.0413
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0520P)^2^+11.4484P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1011
_refine_ls_wR_factor_ref         0.1065
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1692
_reflns_number_total             2085
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            nn1c02022_si_003.cif
_cod_data_source_block           oy8_270k
_cod_database_code               4518728
_shelx_shelxl_version_number     2014/7
_shelx_estimated_absorpt_t_min   0.346
_shelx_estimated_absorpt_t_max   0.471
_shelx_res_checksum              92680
_shelx_hkl_checksum              19766